Active Standard ASTM A564 / A564M | Developed by Subcommittee: A01.17
Book of Standards Volume: 01.03
Historical (view previous versions of standard)
This specification covers bars and shapes of age-hardening stainless steels. Hot-finished or cold-finished rounds, squares, hexagons, bar shapes, angles, tees, and channels are included. These shapes may be produced by hot rolling, extruding, or forging. Type 631 and 632 stainless steels contain a large amount of ferrite in the microstructure and can have low ductility in forgings and large diameter bars. Material of types other than XM-16, XM-25, and Type 630 shall be furnished in the solution-annealed condition, or in the equalized and oven-tempered condition. Types 630, XM-16, and XM-25 may be furnished in the solution-annealed or age-hardened condition. Type UNS S46910 shall be furnished in solution annealed, cold-worked or aged-hardened condition. Shapes may be subjected to either Class A or Class C preparation for removal of visible surface imperfections. The material shall be subjected to tension, impact, and hardness tests.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification2 covers bars and shapes of age-hardening stainless steels. Hot-finished or cold-finished rounds, squares, hexagons, bar shapes, angles, tees, and channels are included; these shapes may be produced by hot rolling, extruding, or forging. Billets or bars for reforging may be purchased to this specification.
1.2 These steels are generally used for parts requiring corrosion resistance and high strength at room temperature, or at temperatures up to 600°F [315°C]; 700°F [370°C] for Type 632; 840°F [450°C] for Type UNS S46910. They are suitable for machining in the solution-annealed condition after which they may be age-hardened to the mechanical properties specified in Section 7 without danger of cracking or distortion. Type XM-25 is machinable in the as-received fully heat treated condition. Type UNS S46910 is suitable for machining in the solution-annealed, cold-worked, and aged-hardened condition.
1.4 The values stated in either inch-pound units or SI (metric) units are to be regarded separately as standards; within the text and tables, the SI units are shown in [brackets]. The values stated in each system are not exact equivalents; therefore, each system must be used independent of the other. Combining values from the two systems may result in nonconformance with the specification.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A314 Specification for Stainless Steel Billets and Bars for Forging
A370 Test Methods and Definitions for Mechanical Testing of Steel Products
A484/A484M Specification for General Requirements for Stainless Steel Bars, Billets, and Forgings
A705/A705M Specification for Age-Hardening Stainless Steel Forgings
A751 Test Methods, Practices, and Terminology for Chemical Analysis of Steel Products
E527 Practice for Numbering Metals and Alloys in the Unified Numbering System (UNS)
Other DocumentsSAE J1086 Recommended Practice for Numbering Metals and Alloys (UNS) Available from Society of Automotive Engineers (SAE), 400 Commonwealth Dr., Warrendale, PA 15096-0001, http://www.sae.org.
ICS Number Code 77.140.60 (Steel bars and rods); 77.140.70 (Steel profiles)